Elucidation of the Na2/3FePO4 and Li2/3FePO4 Intermediate Superstructure Revealing a Pseudouniform Ordering in 2D.
Boucher, Florent; Gaubicher, Joël; Cuisinier, Marine; Guyomard, Dominique; Moreau, Philippe; Journal of the American Chemical Society 136 (2014) 9144–9157; doi:10.1021/ja503622y

data_4121998
_publ_section_title
;
 Elucidation of the Na2/3FePO4 and Li2/3FePO4 Intermediate Superstructure
 Revealing a Pseudouniform Ordering in 2D.
;
_journal_issue                   25
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              9144
_journal_page_last               9157
_journal_paper_doi               10.1021/ja503622y
_journal_volume                  136
_journal_year                    2014
_chemical_formula_iupac          'Na2/3 Fe1 P1 O4'
_chemical_formula_moiety         'Fe3 O12 P3, 2(Na)'
_chemical_formula_structural     'Na2/3 Fe1 P1 O4'
_chemical_formula_sum            'Fe3 Na2 O12 P3'
_chemical_formula_weight         498.44
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90.00000
_cell_angle_beta                 120.7221(7)
_cell_angle_gamma                90.00000
_cell_formula_units_Z            4
_cell_length_a                   18.23736(14)
_cell_length_b                   4.93687(4)
_cell_length_c                   11.96092(11)
_cell_measurement_temperature    293
_cell_volume                     925.769(15)
_computing_cell_refinement       FULLPROF
_computing_data_collection       'MAR345 image plate integration'
_computing_data_reduction        FULLPROF
_computing_structure_refinement  FULLPROF
_diffrn_ambient_temperature      293
_diffrn_detector                 Mar345
_diffrn_detector_type            'Image Plate'
_diffrn_measurement_device_type  2-circle
_diffrn_radiation_monochromator  Si(111)
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.725633
_diffrn_source                   synchrotron
_exptl_absorpt_coefficient_mu    5.603
_exptl_crystal_density_diffrn    3.576
_exptl_crystal_F_000             964
_pd_char_colour                  black
_pd_char_particle_morphology     'nanometric particles'
_pd_instr_location               'Cristal beam line at SOLEIL'
_pd_meas_2theta_range_inc        0.010006
_pd_meas_2theta_range_max        34.99500
_pd_meas_2theta_range_min        0.02500
_pd_meas_number_of_points        3498
_pd_meas_scan_method             step
_pd_proc_2theta_range_inc        0.010006
_pd_proc_2theta_range_max        35.0046
_pd_proc_2theta_range_min        0.0346
_pd_proc_info_excluded_regions   'below 4.7 and from 33.7 to 35.0'
_pd_proc_ls_background_function  'Linearly interpolated'
_pd_proc_ls_profile_function     'Thompson-Cox-Hastings pseudo-Voigt'
_pd_proc_ls_prof_R_factor        0.7571
_pd_proc_ls_prof_wR_expected     1.4109
_pd_proc_ls_prof_wR_factor       1.0972
_pd_proc_wavelength              0.725633
_pd_spec_mounting                'sealed capillarry'
_pd_spec_mount_mode              transmission
_pd_spec_size_axial              10
_pd_spec_size_equat              0.5
_pd_spec_size_thick              0.5
_refine_ls_goodness_of_fit_all   0.777
_refine_ls_number_constraints    5
_refine_ls_number_parameters     103
_refine_ls_number_reflns         662
_refine_ls_number_restraints     12
_refine_ls_R_I_factor            1.3528
_refine_ls_shift/su_max          0.05
_cod_data_source_file            ja503622y_si_002.cif
_cod_data_source_block           Na2/3FePO4
_cod_depositor_comments          'Adding full bibliography for 4121998.cif.'
_cod_original_cell_volume        925.769(13)
_cod_database_code               4121998
_publcif_datablock.id            {aa4dbab4-532c-4727-b889-a1672b10a1dc}
_pd_proc_ls_prof_cr_factor       4.2242
_pd_proc_ls_prof_cwr_factor      3.9046
_pd_proc_ls_prof_cwr_expected    5.0208
_pd_proc_ls_prof_chi2            0.6048
_pd_proc_ls_prof_echi2           0.6048